| ||Format||Pages||Price|| |
|5||$54.00||  ADD TO CART|
|Hardcopy (shipping and handling)||5||$54.00||  ADD TO CART|
|Standard + Redline PDF Bundle||10||$64.00||  ADD TO CART|
Significance and Use
5.1 This test method is of value in rating the tear-propagation resistance of various plastic films and thin sheeting of comparable thickness. For highly extensible film or sheeting the deformation energy of the specimen legs is significantly greater than the tearing energy. The tear-propagation resistance in slightly extensible or non-extensible film or sheeting is distinguished from the tear-propagation resistance in highly extensible film or sheeting by the load-time or load-displacement data, ( and ). The tear-propagation force for slightly extensible or non-extensible material is determined from the average tear force versus the initial and peak force for a highly extensible material.
FIG. 1 Load-Time Chart for Low-Extensible Film
FIG. 2 Load-Time Chart for Highly Extensible Film
5.2 This test method shall be used for specification acceptance testing only after it has been demonstrated that the data for the particular material are acceptably reproducible.
5.3 The data obtained by this test method furnish information for ranking the tear-propagation resistance of plastic films and sheeting of similar composition. Actual use performance may not necessarily correlate with data from this test method. Sets of data from specimens of dissimilar thickness are usually not comparable.
5.4 Before proceeding with this test method, reference should be made to the specification of the material being tested. Any test specimen preparation, conditioning, dimensions, or testing parameters, or combination thereof, covered in the relevant ASTM material specification shall take precedence over those mentioned in this test method. If there are no relevant ASTM material specifications, then the default conditions apply. Table 1 of Classification Systems lists the ASTM materials standards that currently exist.
1.1 This test method covers the determination of the force necessary to propagate a tear in plastic film and thin sheeting (thickness of 1 mm (0.04 in.) or less) by a single-tear method. The method is not applicable for film or sheeting material where brittle failures occur during testing.
Note 1: Film has been arbitrarily defined as sheeting having nominal thickness not greater than 0.25 mm (0.010 in.).
1.2 Constant-Rate-of-Grip Separation Test—This test method employs a constant rate of separation of the grips holding the test specimen.
1.2.1 Specimen extension may be measured in this test method by grip separation.
1.3 The values stated in SI units are to be regarded as standard. The values given in parentheses are provided for information only.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
Note 2: This standard is similar to ISO 6383-1, but is not considered technically equivalent. The specimen size for ISO 6383-1 is larger, and the method specifies different test speeds.
1.5 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D618 Practice for Conditioning Plastics for Testing
D882 Test Method for Tensile Properties of Thin Plastic Sheeting
D883 Terminology Relating to Plastics
D4000 Classification System for Specifying Plastic Materials
D5947 Test Methods for Physical Dimensions of Solid Plastics Specimens
D6988 Guide for Determination of Thickness of Plastic Film Test Specimens
E4 Practices for Force Verification of Testing Machines
E177 Practice for Use of the Terms Precision and Bias in ASTM Test Methods
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
ISO StandardISO 6383-1 Film and SheetingDetermination of Tear Resistance Part 1 Trouser Tear Method Available from American National Standards Institute (ANSI), 25 W. 43rd St., 4th Floor, New York, NY 10036, http://www.ansi.org.
ICS Number Code 83.140.10 (Films and sheets)
UNSPSC Code 13111200(Films); 30265802(Plastic sheet)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D1938-19, Standard Test Method for Tear-Propagation Resistance (Trouser Tear) of Plastic Film and Thin Sheeting by a Single-Tear Method, ASTM International, West Conshohocken, PA, 2019, www.astm.orgBack to Top